ISO 21813 specifies methods for the chemical analysis of fine high purity barium titanate powders used as the raw material for fine ceramics.
ISO 21813 stipulates the determination methods of the barium, titanium, aluminium, cadmium, calcium, cobalt, dysprosium, iron, lead, magnesium, manganese, nickel, niobium, potassium, silicon, sodium, strontium, vanadium, zirconium, carbon, oxygen and nitrogen contents in high purity barium titanate powders. The barium and titanium contents, the major elements, are determined by using an acid decomposition-gravimetric method or an acid decomposition-inductively coupled plasma-optical emission spectrometry (ICP-OES) method. The aluminium, cadmium, calcium, chromium, cobalt, dysprosium, iron, lead, magnesium, manganese, nickel, niobium, potassium, silicon, strontium, vanadium and zirconium contents are simultaneously determined via an acid digestion-ICP-OES method. The nitrogen content is determined by using an inert gas fusion-thermal conductivity method, while that of oxygen is determined via an inert gas fusion-IR absorption spectrometry method. Finally, the carbon content is determined using a combustion-IR absorption spectrometry method or a combustion-conductometry method.
Status: PublishedPublication date: 2019-02
Edition: 1Number of pages: 25
Technical Committee: ISO/TC 206 Fine ceramics
- ICS :
- 81.060.30 Advanced ceramics
This standard contributes to the following Sustainable Development Goal:
Buy this standard
|std 1 124||PDF + ePub|
|std 2 124||Paper|
ISO 21813:2019Stage: 60.60
Got a question?
Check out our FAQs
Monday to Friday - 09:00-12:00, 14:00-17:00 (UTC+1)
Keep up to date with ISO
Sign up to our newsletter for the latest news, views and product information.